|Year : 2021 | Volume
| Issue : 1 | Page : 3
In vitro antimicrobial activity of mineral trioxide aggregate, Biodentine, and calcium-enriched mixture cement against Enterococcus faecalis, Streptococcus mutans, and Candida albicans using the agar diffusion technique
Parinaz Esteki1, Maryam Zare Jahromi2, Arezoo Tahmourespour3
1 Graduated of Dental School, Islamic Azad University, Isfahan, Iran
2 Department of Endodontics, Dental School, Islamic Azad University, Isfahan, Iran
3 Department of Basic Medical Sciences, Dental School, Islamic Azad University, Isfahan (Khorasgan) Branch, Isfahan, Iran
|Date of Submission||17-Feb-2020|
|Date of Acceptance||21-Oct-2020|
|Date of Web Publication||23-Feb-2021|
Dr. Maryam Zare Jahromi
Department of Endodontics, Dental School, Islamic Azad University, Isfahan (Khorasgan) Branch, Isfahan
Source of Support: None, Conflict of Interest: None
Background: This study assessed the antimicrobial activity of Biodentine, mineral trioxide aggregate (MTA), and calcium-enriched mixture (CEM) cement against Enterococcus faecalis, Streptococcus mutans , and Candida albicans.
Materials and Methods: In this in vitro study, microbial suspensions were inoculated onto agar plates. The antimicrobial effects of MTA, Biodentine and CEM cement were assessed against E. faecalis, S. mutans, and C. albicans by the agar diffusion test. In each experimental group, 7 plates containing 3 wells were prepared and immediately filled with freshly mixed cements. Positive and negative control plates were prepared with/without the bacterial suspension, respectively. After 2 h of preincubation at room temperature, the plates were incubated at 37°C for 24 h. The diameter of growth inhibition zones was measured after 24 h. Data were analyzed using ANOVA and Tukey's test (α = 0.05).
Results: Biodentine showed strong antimicrobial activity against all three microorganisms with an average inhibition zone of 9.10 mm. The inhibitory effect of Biodentine on E. faecalis and C. albicans was significantly superior to that of the other two cements (P < 0.05). MTA and CEM cement showed significantly higher antimicrobial activity against S. mutans (P < 0.05). The antimicrobial effects of Biodentine on S. mutans and E. faecalis were significantly greater than on C. albicans (P < 0.05).
Conclusion: All cements revealed antimicrobial properties against the tested microbial strains. Biodentine had stronger antimicrobial effects against E. faecalis and C. albicans compared with MTA and CEM cement. Furthermore, the largest inhibition zones around all three cements belonged to S. mutans.
Keywords: Biodentine, calcium-enriched mixture cement, Candida albicans, Enterococcus faecalis, mineral trioxide aggregate
|How to cite this article:|
Esteki P, Jahromi MZ, Tahmourespour A. In vitro antimicrobial activity of mineral trioxide aggregate, Biodentine, and calcium-enriched mixture cement against Enterococcus faecalis, Streptococcus mutans, and Candida albicans using the agar diffusion technique. Dent Res J 2021;18:3
|How to cite this URL:|
Esteki P, Jahromi MZ, Tahmourespour A. In vitro antimicrobial activity of mineral trioxide aggregate, Biodentine, and calcium-enriched mixture cement against Enterococcus faecalis, Streptococcus mutans, and Candida albicans using the agar diffusion technique. Dent Res J [serial online] 2021 [cited 2021 Mar 8];18:3. Available from: https://www.drjjournal.net/text.asp?2021/18/1/3/310032
| Introduction|| |
Microorganisms are the main culprits responsible for the development of pulpal and periapical diseases and can cause endodontic treatment failures. Provision of an effective seal to prevent recontamination as well as successful elimination or reduction of microorganisms in the root canal system can positively affect the outcome of endodontic treatment. The endodontic procedural steps such as chemomechanical instrumentation, root canal irrigation, application of intracanal medicaments, and sealing of the pulp chamber eliminate the microorganisms and enhance regeneration of periapical tissues. After chemomechanical preparation, however, some bacteria may remain in ramifications and dentinal tubules and lead to treatment failure. There is no definite strategy to completely eliminate residual bacteria. Moreover, many of the currently available biomaterials may not create an ideal seal. Thus, it is imperative to use endodontic cements with the ability to inhibit bacterial growth. Therefore, the antimicrobial properties of these biomaterials should be investigated. The agar diffusion test is the most widely used technique to assess the antimicrobial properties of dental materials.
Mineral trioxide aggregate (MTA) was first introduced by Torabinejad et al. Its application has been successful for furcal and lateral root surface perforation repairs, as well as root-end filling, vital pulp capping, and also as an apical plug in apexification. MTA is supplied in the form of a powder with fine hydrophilic particles that form a colloidal gel in the presence of water. It is solidified and forms hard cement within nearly 4 h. MTA has many advantages such as osteogenic and regeneration potential, good marginal sealability, bioactivity, biocompatibility, and antibacterial effects., However, long setting time, high cost, poor handling properties, and tooth discoloration are its main drawbacks.,,
Calcium-enriched mixture (CEM) cement was introduced in 2006 and contains different calcium compounds. The mixed CEM cement consists of water-soluble calcium and phosphate, which immediately lead to the formation of hydroxyapatite during and after the setting period. This cement is biocompatible and its clinical application is similar to that of MTA; however, their chemical compositions are different. This cement creates an effective seal and provokes the healing of hard tissue as does the MTA.,, However, in comparison with MTA, it has a shorter setting time, lower cost, lower tooth discoloration potential and easier handling.,, Moreover, CEM cement potentially prevents bacterial growth.,,
Biodentine is a novel calcium-silicate based endodontic cement. Its powder mainly consists of tricalcium and dicalcium silicate, calcium carbonate and zirconium dioxide as a contrast medium. The liquid contains calcium chloride, which accelerates the setting reactions and is used as a water-reducing agent in aqueous solutions with a mixture of polycarboxylate and sets in 12 min.,, Biodentine is a dentine replacement material, which can be used for filling of deep and extensive coronal caries, restoring of deep cervical and radicular lesions, pulpotomy and pulp capping, furcal and root perforation repair, management of internal and external resorptions, apexification, and surgical root-end filling.,
A number of studies have investigated the antimicrobial effects of MTA, Biodentine and CEM cement. In a study by Bhavana et al., in 2015, Biodentine showed stronger inhibitory effect than MTA on Streptococcus mutans, Enterococcus faecalis and Candida albicans. Moreover, Asgary et al., in 2007, reported that antibacterial properties of CEM cement against E. faecalis were higher than those of MTA. According to Koruyucu et al., in 2015, Biodentine and MTA showed similar antibacterial effects against E. faecalis.
The aim of this experimental study was to compare the antimicrobial activity of MTA, Biodentine and CEM cement against E. faecalis, S. mutans and C. albicans by the agar diffusion technique.
| Materials and Methods|| |
In this in vitro experimental study, the MTA (Angelus, Brazil), Biodentine (Septodont, France) and CEM cement (Yektazist, Iran) were individually mixed according to the manufacturers' instructions. The antimicrobial effects of these endodontic cements were evaluated against three reference strains namely E. faecalis (ATCC 29212), S. mutans (ATCC 35668), and C. albicans (ATCC 10231) by the agar diffusion method. The strains were obtained from the Department of Microbiology, Faculty of Dentistry, Azad University, Isfahan (Khorasgan) branch. Trypticase soy broth (Merck, Germany) and Sabouraud dextrose broth (Merck, Germany) were used for activation of microorganisms. Then, the overnight cultures of microorganisms were diluted by sterile trypticase soy broth and Sabouraud dextrose broth to obtain a suspension with 0.5 McFarland standard turbidity, which corresponds to a concentration of 1.5 × 108 CFUs/mL. All microbial strains were confirmed with growth characteristics and Gram-staining.
Standard suspensions of E. faecalis and C. albicans were inoculated onto Mueller-Hinton agar plates (Merck, Germany), and S. mutans suspension was inoculated onto blood agar plates (Merck, Germany) with sterile cotton swabs using the lawn culture method. Three wells, 4 mm deep and 5 mm in diameter, were prepared on each plate with a sterile Pasteur pipette, and immediately filled with freshly mixed test materials. For prediffusion of the materials, the plates were placed at room temperature for 2 h. Then, all the plates were incubated at 37°C and assessed after 24 h.,
The total number of plates, including the test plates and positive and negative controls, was 26. The plates were randomly divided into three groups for each microorganism. In each group, 7 plates containing three wells for testing each of the three cements were considered. The antimicrobial effect of each cement was tested seven times against each microorganism. Positive and negative control plates were prepared with and without the bacterial suspension, respectively and kept for the same incubation time under similar conditions. All experiments were performed in sterile conditions.
The diameter of microbial growth inhibition zones was measured by a digital caliper with 0.01 mm accuracy by an independent observer. Data were analyzed using SPSS software version 22 (SPSS Inc., Chicago, IL, USA), and the results were expressed as means and standard deviations. To compare the differences between the materials, data were analyzed statistically by one-way ANOVA and Tukey's post hoc test for multiple comparisons. P < 0.05 was considered statistically significant.
| Results|| |
The positive control groups showed microbial growth, while there was no sign of microbial growth in the negative control groups. Growth of all microbial species was inhibited by all the tested materials. [Table 1] shows the antimicrobial activity of the cements against all tested microorganisms, which was evaluated by determining the mean and standard deviation of growth inhibition zones (mm) after 24 h. The greatest antimicrobial effect belonged to Biodentine and CEM cement against S. mutans and the least antimicrobial effect belonged to CEM cement against E. faecalis.
|Table 1: Antimicrobial activity of the cements against the three microbial species|
Click here to view
The maximum mean diameter of growth inhibition zone of E. faecalis and C. albicans was found around Biodentine, while the growth inhibition zones around MTA and CEM cement were smaller.
[Table 2],[Table 3],[Table 4] show pairwise comparisons of the cements against the three microorganisms, done by the Tukey's test. The results showed that the antimicrobial activity of Biodentine against E. faecalis was significantly higher than that of MTA and CEM cement (P < 0.001). Moreover, the antifungal activity of Biodentine against C. albicans was significantly greater than that of MTA (P < 0.001) and CEM cement (P = 0.002). In this study, the antimicrobial effect of CEM cement against S. mutans was significantly higher than that of MTA (P = 0.038), while there was no significant difference between Biodentine and CEM cement (P = 0.958). Although the antimicrobial effect of Biodentine and CEM cement against S. mutans was superior to the effect of MTA, the difference between Biodentine and MTA was close to the significant level (P = 0.066). Furthermore, for all three cements, the maximum mean growth inhibition zone belonged to S. mutans.
| Discussion|| |
An ideal endodontic cement should have bacteriostatic or bactericidal properties. Furthermore, root-end filling biomaterials should inherently have antimicrobial effects because many bacteria causing primary infections or treatment-resistant microorganisms may remain in the root canal system in case of persistent endodontic infections. In chronic or refractory periapical lesions, facultative bacteria, and yeasts are the most prevalent and predominant microorganisms.
E. faecalis forms a minor part of the microbial flora in uninstrumented canals, while it is a main etiologic factor for periradicular lesions that develop following the endodontic treatment. It has been isolated from 22% to 77% of teeth with failed endodontic treatments. E. faecalis is resistant to high pH and has the ability to invade the dentinal tubules. Thus, it is highly resistant to intracanal medicaments., S. mutans can have significant effects on both the initial and secondary pulpal lesions. C. albicans is capable of creating a biofilm on various surfaces and may be found in cases of persistent and secondary infections. For the aforementioned reasons, the antimicrobial activity of the three abovementioned microorganisms was tested against three commonly used endodontic cements in this study.
The agar diffusion test, which is the most common method for the assessment of antimicrobial activity, was used in this study. The diffusion capability of the material through the medium greatly affects the outcome of the agar diffusion test. However, the results of agar diffusion test also depend on many factors, such as the selection of microorganisms and the agar medium used, standardization of the concentration of microbial suspensions, incubation times and measurement of growth inhibition zones. The incubation period was considered 24 h in this study; also, the microbial suspension was diluted to 0.5 McFarland standard concentration, which was similar to the previous studies., Moreover, according to similar previous studies, all plates were maintained at room temperature for 2 h for prediffusion of materials., In this study, attempts were made to standardize the testing conditions to minimize the effect of confounders.
In this study, the antimicrobial properties of Biodentine, MTA and CEM cement were assessed, and freshly mixed materials were transferred into agar plates immediately because the antimicrobial efficacy of materials is affected by their degree of polymerization. Our results showed that all the test materials had antimicrobial effects against the tested microorganisms. The antimicrobial characteristics of MTA may be due to its alkalinity. A pH higher than nine can reversibly or irreversibly deactivate cellular membrane enzymes of the microorganisms, leading to loss of their biological activity. The initial pH of the freshly mixed MTA is 10.2, but it reaches 12.5 after 3 h, probably due to the release of calcium hydroxide during the hydration process.
The main constituents of CEM cement include alkaline earth metal hydroxides and oxides (e.g., calcium hydroxide and calcium oxide), calcium silicate, and calcium phosphate. The pH of CEM cement is around 10.71 after 1 h. During and after mixing with its liquid, the hydration reactions occur, which produce calcium hydroxide. When CEM cement is transferred into agar plates and contacts the medium, calcium hydroxide dissociates into calcium and hydroxyl ions, which raise the pH and calcium levels. Calcium hydroxide with a pH of 12.5 is a major CEM cement byproduct.,, This can explain the optimal antimicrobial activity of this cement, at least in part. Another possible reason can be the superior diffusion properties of antimicrobial constituents of CEM cement.
Biodentine has greater mechanical properties and less solubility. It provides a tighter seal, has more convenient handling properties and requires less time to set in comparison with other materials such as MTA. The findings of the present study showed that Biodentine had better antifungal and antibacterial effects than MTA. Antimicrobial properties of Biodentine are strongly related to its calcium release and alkalinity. During the hydration process of the cement, colloidal gel is formed, which leads to the release of calcium hydroxide that prevents bacterial growth. Furthermore, the pH of Biodentine increases to 12.5 during setting; therefore, bacterial growth is inhibited, and the surrounding areas are disinfected.
None of the previous studies has compared the antimicrobial activity of MTA, Biodentine and CEM cement. Unlike this study, Estrela et al. demonstrated that MTA did not show any antimicrobial activity against C. albicans and E. faecalis. Moreover, Torabinejad et al. revealed that MTA was not effective against E. faecalis, which contradicted the results of this study. Our results revealed that Biodentine had greater antimicrobial efficacy against C. albicans and E. faecalis than the other two cements. Chopra et al. indicated that the growth inhibition zones of these two microorganisms around Biodentine were significantly larger than the area around MTA, which was consistent with the results of this study. Furthermore, Jose et al., demonstrated that Biodentine had significantly superior antimicrobial activity compared with MTA, which was confirmed by the results of the present study. Similar to the present study, Bhavana et al. concluded that antimicrobial activity of Biodentine against E. faecalis, S. mutans and C. albicans was greater than that of MTA. In addition, in the study by Bhavana, the inhibition zone diameters of S. mutans around Biodentine and MTA were significantly greater than around E. faecalis and C. albicans, which is parallel to the results of the current study on MTA. Nourzadeh et al., in 2019, discussed that CEM cement had a higher inhibitory effect on E. faecalis than Biodentine, while the present study suggested a stronger antibacterial activity than CEM cement against E. faecalis. It should be mentioned that the discrepancy between the results of studies can be attributed to the available nutrients, incubation period, oxygen pressure level, techniques of assessment, and diverse laboratory set-ups used.
| Conclusion|| |
- All three cements had growth inhibitory effects on the three types of microorganisms tested
- Compared with MTA, Biodentine showed greater inhibitory effects against E. faecalis and C. albicans, which are resistant microorganisms in endodontic treatment
- The greatest inhibition zone in all three materials was related to S. mutans.
Biodentine with its potent antimicrobial effect can be considered as an appropriate alternative to MTA and CEM cement in endodontic treatment. Due to the lack of studies to compare the antimicrobial properties of Biodentine, MTA and CEM cement, further studies are recommended before introducing Biodentine as an ideal material for endodontic treatments.
Financial support and sponsorship
Conflicts of interest
The authors of this manuscript declare that they have no conflicts of interest, real or perceived, financial or non-financial in this article.
| References|| |
Fouad AF, Zerella J, Barry J, Spångberg LS. Molecular detection of Enterococcus
species in root canals of therapy-resistant endodontic infections. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 2005;99:112-8.
Torabinejad M, Hong CU, Pitt Ford TR, Kettering JD. Antibacterial effects of some root end filling materials. J Endod 1995;21:403-6.
Leonardo MR, Tanomaru Filho M, Silva LA, Nelson Filho P, Bonifácio KC, Ito IY. In vivo
antimicrobial activity of 2% chlorhexidine used as a root canal irrigating solution. J Endod 1999;25:167-71.
Orstavik D. Antibacterial properties of root canal sealers, cements and pastes. Int Endod J 1981;14:125-33.
Cobankara FK, Altinöz HC, Ergani O, Kav K, Belli S. In vitro
antibacterial activities of root-canal sealers by using two different methods. J Endod 2004;30:57-60.
Torabinejad M, Watson TF, Pitt Ford TR. Sealing ability of a mineral trioxide aggregate when used as a root end filling material. J Endod 1993;19:591-5.
Torabinejad M, Hong CU, McDonald F, Pitt Ford TR. Physical and chemical properties of a new root-end filling material. J Endod 1995;21:349-53.
Saunders WP. A prospective clinical study of periradicular surgery using mineral trioxide aggregate as a root-end filling. J Endod 2008;34:660-5.
Parirokh M, Torabinejad M. Mineral trioxide aggregate: A comprehensive literature review Part I: Chemical, physical, and antibacterial properties. J Endod 2010;36:16-27.
Dammaschke T, Gerth HU, Züchner H, Schäfer E. Chemical and physical surface and bulk material characterization of white ProRoot MTA and two Portland cements. Dent Mater 2005;21:731-8.
Meraji N, Bolhari B, Sefideh MR, Niavarzi S. Prevention of tooth discoloration due to calcium-silicate cements: A review. Dent Hypotheses 2019;10:4-8. [Full text]
Asgary S, Eghbal MJ, Parirokh M, Torabzadeh H. Sealing ability of three commercial mineral trioxide aggregates and an experimental root-end filling material. Iran Endod J 2006;1:101-5.
Asgary S, Parirokh M, Eghbal MJ, Ghoddusi J. SEM evaluation of pulp reaction to different pulp capping materials in dog's teeth. Iran Endod J 2006;1:117-23.
Yavari HR, Samiei M, Shahi S, Aghazadeh M, Jafari F, Abdolrahimi M, et al
. Microleakage comparison of four dental materials as intra-orifice barriers in endodontically treated teeth. Iran Endod J 2012;7:25-30.
Nosrat A, Asgary S, Eghbal MJ, Ghoddusi J, Bayat-Movahed S. Calcium-enriched mixture cement as artificial apical barrier: A case series. J Conserv Dent 2011;14:427-31.
] [Full text]
Asgary S, Ahmadyar M. Vital pulp therapy using calcium-enriched mixture: An evidence-based review. J Conserv Dent 2013;16:92-8.
] [Full text]
Kazem M, Eghbal MJ, Asgary S. Comparison of bacterial and dye microleakage of different root-end filling materials. Iran Endod J 2010;5:17-22.
Žižka R, Šedý J, Gregor L, Voborná I. Discoloration after regenerative endodontic procedures: A critical review. Iran Endod J 2018;13:278-84.
Hasan Zarrabi M, Javidi M, Naderinasab M, Gharechahi M. Comparative evaluation of antimicrobial activity of three cements: New endodontic cement (NEC), mineral trioxide aggregate (MTA) and Portland. J Oral Sci 2009;51:437-42.
Razmi H, Aminsobhani M, Bolhari B, Shamshirgar F, Shahsavan S, Shamshiri AR. Calcium enriched mixture and mineral trioxide aggregate activities against Enterococcus faecalis
in presence of dentin. Iran Endod J 2013;8:191-6.
Asgary S, Kamrani FA. Antibacterial effects of five different root canal sealing materials. J Oral Sci 2008;50:469-74.
Nowicka A, Lipski M, Parafiniuk M, Sporniak-Tutak K, Lichota D, Kosierkiewicz A, et al
. Response of human dental pulp capped with biodentine and mineral trioxide aggregate. J Endod 2013;39:743-7.
Laurent P, Camps J, About I. Biodentine™ induces TGF-β1 release from human pulp cells and early dental pulp mineralization. Int Endod J 2012;45(5):439-48.
Tran XV, Gorin C, Willig C, Baroukh B, Pellat B, Decup F, et al
. Effect of a calcium-silicate-based restorative cement on pulp repair. J Dent Res 2012;91:1166-71.
Camilleri J, Sorrentino F, Damidot D. Investigation of the hydration and bioactivity of radiopacified tricalcium silicate cement, Biodentine and MTA Angelus. Dent Mater 2013;29:580-93.
Camilleri J. Investigation of Biodentine as dentine replacement material. J Dent 2013;41:600-10.
Bhavana V, Chaitanya KP, Gandi P, Patil J, Dola B, Reddy RB. Evaluation of antibacterial and antifungal activity of new calcium-based cement (Biodentine) compared to MTA and glass ionomer cement. J Conserv Dent 2015;18:44-6.
] [Full text]
Asgary S, Akbari Kamrani F, Taheri S. Evaluation of antimicrobial effect of MTA, calcium hydroxide, and CEM cement. Iran Endod J 2007;2:105-9.
Koruyucu M, Topcuoglu N, Tuna EB, Ozel S, Gencay K, Kulekci G, et al
. An assessment of antibacterial activity of three pulp capping materials on Enterococcus faecalis
by a direct contact test: An in vitro
study. Eur J Dent 2015;9:240-5.
] [Full text]
Jose J, Shoba K, Tomy N, Aman S. Comparative evaluation of antimicrobial activity of Biodentine and MTA against Enterococcus faecalis
an in vitro
study. Int J Dent Res 2016;4:16-8.
Stuart CH, Schwartz SA, Beeson TJ, Owatz CB. Enterococcus faecalis
: Its role in root canal treatment failure and current concepts in retreatment. J Endod 2006;32:93-8.
Zhang H, Pappen FG, Haapasalo M. Dentin enhances the antibacterial effect of mineral trioxide aggregate and bioaggregate. J Endod 2009;35:221-4.
Parirokh M, Talebizad M, Forghani FR, Haghdoost AA, Asgary S, Eghbal MJ, et al
. Fluoride varnish as root canal sealer: A scanning electron microscopy and bacterial penetration study. Iran Endod J 2015;10:64-8.
Hahn CL, Best AM, Tew JG. Cytokine induction by Streptococcus mutans
and pulpal pathogenesis. Infect Immun 2000;68:6785-9.
Siqueira JF Jr., Sen BH. Fungi in endodontic infections. Oral Surg Oral Med Oral Pathol Oral Radiol Endod 2004;97:632-41.
Leonardo MR, da Silva LA, Tanomaru Filho M, Bonifácio KC, Ito IY. In vitro
evaluation of antimicrobial activity of sealers and pastes used in endodontics. J Endod 2000;26:391-4.
Fraga RC, Siqueira JF Jr., de Uzeda M. In vitro
evaluation of antibacterial effects of photo-cured glass ionomer liners and dentin bonding agents during setting. J Prosthet Dent 1996;76:483-6.
Sipert CR, Hussne RP, Nishiyama CK, Torres SA. In vitro
antimicrobial activity of Fill Canal, Sealapex, Mineral Trioxide Aggregate, Portland cement and EndoRez. Int Endod J 2005;38:539-43.
Fridland M, Rosado R. Mineral trioxide aggregate (MTA) solubility and porosity with different water-to-powder ratios. J Endod 2003;29:814-7.
Estrela C, Sydney GB, Bammann LL, Felippe Júnior O. Mechanism of action of calcium and hydroxyl ions of calcium hydroxide on tissue and bacteria. Braz Dent J 1995;6:85-90.
Fridland M, Rosado R. MTA solubility: A long term study. J Endod 2005;31:376-9.
Amini Ghazvini S, Abdo Tabrizi M, Kobarfard F, Akbarzadeh Baghban A, Asgary S. Ion release and pH of a new endodontic cement, MTA and Portland cement. Iran Endod J 2009;4:74-8.
Asgary S, Shahabi S, Jafarzadeh T, Amini S, Kheirieh S. The properties of a new endodontic material. J Endod 2008;34:990-3.
Popovics S. Strength and Related Properties of Concrete: A Quantitative Approach. New York: John Wiley & Sons; 1998.
Chopra MS, Gulve MN. Evaluation of the antibacterial and antifungal activity of three retrograde filling materials: An in vitro
study. Int J Contem Med Res 2016;3:2286-8.
Estrela C, Bammann LL, Estrela CR, Silva RS, Pécora JD. Antimicrobial and chemical study of MTA, Portland cement, calcium hydroxide paste, Sealapex and Dycal. Braz Dent J 2000;11:3-9.
Nourzadeh M, Amini A, Fakoor F, Asgary S. Antimicrobial activity of calcium-enriched mixture cement and biodentine on Enterococcus faecalis
: An in vitro
study. Iran Endod J 2019;14:18-22.
[Table 1], [Table 2], [Table 3], [Table 4]